# chapter 4. permeability, diffusivity, and solubility of ... chapter 4. permeability, diffusivity,...

Post on 11-Mar-2020

0 views

Embed Size (px)

TRANSCRIPT

29

Chapter 4. Permeability, Diffusivity, and Solubility of Gas and Solute Through Polymers

Introduction

The diffusion of small molecules into polymers is a function of both the polymer and the

diffusant. Factors which influence diffusion include: (1) the molecular size and physical state of

the diffusant; (2) the morphology of the polymer; (3) the compatibility or solubility limit of the

solute within the polymer matrix; (4) the volatility of the solute; (5) and the surface or interfacial

energies of the monolayer films (1-4). Researchers have attempted to explain specific

mechanisms by which diffusion occurs in polymeric systems, but there is no unified theory to

explain this phenomenon (5).

Formulation of the gas transport phenomena through polymer membranes is directed in

two areas: (1) development of quantitative theories based on the thermodynamics and kinetic

properties of the gas-polymer system, and (2) experimental study of gas transport through

various polymers. Most quantitative theories are primarily based on regular polymer solution

theories. Empirical studies observe behaviors for gas-polymer systems and then correlate these

findings to known phenomenological models. Based on the focus of these empirical studies,

either microscopic (molecular) or macroscopic (continuum) theories are employed (6).

Theory of Gas Permeation and Diffusion Through Polymer Membranes

Fundamentals

The first study of gas permeation through a polymer was conducted by Thomas Graham

in 1829 (7). Graham observed a loss in volume of a wet pig bladder inflated with CO2. In 1866,

Graham formulated the solution diffusion process, where he postulated that the permeation

process involved the dissolution of penetrant, followed by transmission of the dissolved species

through the membrane. The other important observations made at the time were:

1) Permeation was independent of pressure.

2) Increase in temperature lead to decrease in penetrant solubility, but made

the membrane more permeable.

3) Prolonged exposure to elevated temperature affected the retention capacity

of the membrane.

30

4) Differences in the permeability could be exploited for application in gas

separations.

5) Variation in membrane thickness altered the permeation rate but not the

separation characteristics of the polymer.

Fick in 1855, by analogy to Fourier’s law of heat conduction, proposed the law of mass

diffusion which is stated as, …”the mathematical theory of diffusion in isotropic substances is

based on the hypothesis that the rate of transfer of diffusing substances through unit area of a

section is proportional to the concentration gradient measured normal to the section” (8). Fick’s

first law of diffusion is mathematically expressed as:

' qor For

x CDJ

∂ ∂−= (1)

where J, F, or q is the rate of transfer per unit area of section, C is the concentration of diffusing

substances, and x is the space co-ordinate measured normal to the section. If F and C are both

expressed in terms of the same unit of quantity, D is then independent of the unit and has

dimensions length2 time-1.

Once the mass-balance of an element is taken into account, equation (1) can be used to

derive the fundamental differential equation of diffusion: (8)

∂ ∂+

∂ ∂+

∂ ∂=

∂ ∂

2

2

2

2

2

2

z C

y C

x CD

t C . (2)

In polymeric and non-homogeneous systems, the diffusion coefficient largely depends on the

concentration. The diffusion coefficient in polymeric and non-homogeneous systems varies

from point to point and equation (2) is more accurately expressed: (8)

∂ ∂

= ∂ ∂

∂ ∂

+

∂ ∂

∂ ∂

+

∂ ∂

∂ ∂

C t x

D C x y

D C y z

D C z

(3)

31

where D is a function of x, y, z and C. In most applications, diffusion is restricted to one

direction. For example, many times a gradient of concentration is present and diffusion only

occurs along the x-axis. In these cases, equations (2) and (3) can be reduced to: (8)

∂ ∂

= ∂ ∂

C t

D C x

2

2 (4)

and

∂ ∂

∂ ∂=

∂ ∂

x CD

xt C , respectively. (5)

Equations (4) and (5) are commonly referred to as Fick’s second law of diffusion.

In the late 1870’s, Stefan and Exner demonstrated that gas permeation through a soap

membrane was proportional to the product of solubility coefficient (S) and Fick’s diffusion

coefficient (D). Based on the findings of Stefan and Exner, von Wroblewski constructed a

quantitative solution to the Graham’s solution-diffusion model. The dissolution of gas was based

on Henry’s law of solubility, where the concentration of the gas in the membrane was directly

proportional to the applied gas pressure: (7)

S CP = (6)

where P is the permeability coefficient.

Wroblewski further showed that under steady state conditions, and assuming diffusion

and solubility coefficients to be independent of concentration, the gas permeation flux can be

expressed as: (7)

∆=

− ⋅⋅=

l pP

l pp

SDJ pf (7)

32

where (pf) and (pp) are the upstream and downstream pressures imposed on a membrane, (∆p/l) is

the applied pressure gradient across the membrane thickness (l), and P is defined as the gas

permeability of the membrane. A schematic representation of gas transport through a membrane

is shown in Figure 1. The gas permeability of a membrane is often expressed in Barrers, where 1

Barrer = 10-10 (cm3(STP) / cm. sec. cmHg).

In 1920, Daynes showed that it was impossible to evaluate both diffusion and solubility

coefficients by steady-state permeation experiments. He presented a mathematical solution using

Fick’s second law of diffusion, equations (4) and (5), for calculating the diffusion coefficient,

which was assumed to be independent of concentration: (7)

2

2

x CD

t C

∂ ∂=

∂ ∂ . (8)

This “time lag method” is still the most common method for estimating the gas diffusion

coefficient.

Permeation Models and Methods of Calculation

Steady State Model

Many mathematical models used to describe diffusion assume steady state conditions.

Steady state conditions assume that diffusant concentrations remain constant at all points on each

side or surface of a plastic sheet or membrane. Provided the diffusion coefficient is constant,

Fick’s second law of diffusion, equation (4), reduces to: (8)

d C dx

2

2 0= . (9)

Integrating equation (9) twice with respect to x and introducing the conditions at x=0 and l, one

obtains: (8)

l x

CC CC =

− −

12

1 . (10)

33

The concentration changes linearly from C1 to C2 through a plastic sheet or membrane and the

rate of transfer for a diffusing substance is the same across all sections. Therefore, the rate of

transfer per unit area of section is calculated by: (8)

( ) l

CCD dx dCDJ 21

− =−= . (11)

If the thickness and the surface concentrations of the diffusant are known, the diffusion

coefficient can be extrapolated from flow rate.

In systems where a gas or vapor is the diffusant, the surface concentration may not be

known. In gas and vapor systems, the rate of diffusant transfer is expressed in terms of vapor

pressures, ρ1, ρ2, by the following equation: (8)

( ) l

P J 21

ρρ − = (12)

where P is the permeability coefficient. Henry’s law of solubility, equation (6), states that a

linear relationship exists between the external vapor pressure and the corresponding

concentration within the surface of the plastic sheet or membrane (8). The relationship in

equation (6) is commonly extrapolated from a linear sorption isotherm. If one assumes the

diffusion coefficient to be constant, the relationship between the diffusion coefficient, the

permeation coefficient, and the solubility coefficient simplifies to: (8).

SDP ⋅= . (13)

In closing, if the rate of diffusion is empirically determined and the solubility coefficient for the

diffusant is known, the permeation and diffusion coefficients are easily calculated from

equations (12) and (13).

34

Time Lag Method Assuming

Recommended